MEMORIAL DESCRITIVO PARA A CONTRATAÇÃO DE SERVIÇOS DE OPERAÇÃO, MANUTENÇÃO E MONITORAMENTO DE SISTE-
HISTÓRICO E SITUAÇÃO FÍSICA 2.1.
3. ESCOPO DOS SERVIÇOS ESCOPO DOS SERVIÇOS ESCOPO DOS SERVIÇOS ESCOPO DOS SERVIÇOS
5.2.1 Choice of normal load
The bulk single-crystal sapphire (0001) sample was taken for the investigation. It has well known mechanical properties, i.e. the Young’s modulus of 420 GPa and yield strength of 28.0 GPa at the Poisson’s ratio of 0.234 .
To decrease the probability of plastic deformation during lateral force application the normal load should be less than the critical value for plasticity onset at the normal indentation. On the other hand, this normal load should be enough for the achievement of the critical tensile stress for fracture formation.
According to the von Mises stress simulation by the software Elastica the application of 400 mN normal load to bulk sapphire sample corresponds to the elastic measurements at 10.5 µm diamond spherical indenter. The maximum von Mises stress is equal to 27.1 GPa, i.e. it is less than the yield strength of sapphire.
The experimental application of this force by means of the loading-unloading cycle, which is similar to the cycle presented in Fig. 3.2a, confirms the elastic nature of measurements (see Fig.
5.4). Thus, the normal load of 400 mN was used for the study of the fracture formation in single-crystal sapphire.
0.00 0.05 0.10 0.15 0.20 0.25 0.30 0.35 0.40 0.45 0
Normal displacement (µm) Measurement
Figure 5.4. Normal load-displacement curves. The loading part of curves completely agrees with the unloading part of curves as in the case of elastic deformation.
5.2.2 Experimental procedure
The normal and LFU forces were simultaneously applied to the sample according to the force cycles presented in Fig. 5.5.
0 50 100 150 200 250 300 350 400 450 500
Figure 5.5. Normal and LFU force cycles.
Chapter 5. Determination of critical tensile stress for crack formation in single-crystal sapphire As is shown in Fig. 5.5 the normal force increases linearly within 75 s up to the maximal value of 400 mN (1). When the maximal value of normal force is achieved the LFU force is im-mediately started. The LFU force increases within 120 s linearly up to 100 mN (2-3-4) and de-creases within 120 s linearly to zero (5).
5.2.3 Failure detection in lateral force-displacement curves
As the result of the combined application of normal and lateral forces two types of lateral force-displacement curves have been obtained (see Fig. 5.6).
-160 -80 0 80 160 240 320 400 480 560 640
Figure 5.6. Lateral force-displacement curves. The sudden increasing of lateral displacement is observed for both curves in the dotted circle. The numeration of the parts of curves corresponds to the numeration in Fig. 5.5.
The description of behaviour of these lateral force-displacement curves considerably differs from the description of standard curves presented in section 4.5.3. During the initial lateral hold period (1) the lateral force is kept zero. The normal load is increased to its maximal value of 400 mN and kept constant afterwards. The significant shift of the zero position by 100 ± 5 nm in negative direction of lateral displacement axis and by 2.1 ± 0.1 mN in positive direction of lat-eral force axis can be explained by the influence of the factors mentioned in section 4.2.1 at the significant normal load of 400 mN.
At the beginning of lateral loading (2) a lateral displacement is not observed due to the stick-ing of indenter to the sample surface. The bendstick-ing of indenter shaft occurs at the beginnstick-ing of this period.
At the achievement of nominal lateral force of 16.8 ± 0.1 mN for both types of curves (3) the momentary increase of lateral displacement is observed in the direction of lateral force applica-tion. The most probable explanation of this sudden significant increase of lateral displacement is
a failure. For both types of curves the absolute value of sudden lateral displacement is 250 ± 6 nm.
During further lateral loading (4) the behaviour of curves becomes different. For the curve of type 1 the lateral force rises up to the maximum value of 18.8 ± 0.1 mN without a significant lateral displacement. Thus, after the sudden increase of lateral displacement connected with the failure the indenter sticks again to the sample surface. As a proof of this assertion it should be noted that the ratio of lateral and normal forces of 0.047, which is achieved at the end of this period, is less than the static friction coefficient of 0.052 for sapphire against diamond (see Table 7.1). On the other hand, during lateral displacement the lateral force of 12.9 ± 0.7 mN is ob-served for the curve of type 2. The most probable explanation of such a behaviour is that after the failure the indenter slides along the sample surface.
During the lateral unloading (5) the indenter sticks to the sample surface due to adhesion. A lateral displacement is not observed. The bending of indenter shaft changes in the opposite direc-tion at the beginning of this period. Most probably, some slope of curve at this period as well as slope at period 2 has artificial nature.
Thus, according to Fig. 5.6 the failure is detected at the application of lateral force of 14.7 ± 0.1 mN, which is the difference between detected force of 16.8 ± 0.1 mN and force of 2.1 ± 0.1 mN corresponding to the zero position of indenter.
5.2.4 Failure detection in normal displacement-time curves
As was mentioned in section 4.5.4 the normal displacement-time curves allow to get the ad-ditional information about lateral force application. Thus, two normal displacement-time curves were obtained for both types of the lateral force-displacement curves presented above (see Fig.
Figure 5.7. Normal displacement versus time during normal hold period at the maximum normal load (after thermal drift correction). The sudden change of normal displacement is observed for both curves in the dotted oval.
Chapter 5. Determination of critical tensile stress for crack formation in single-crystal sapphire Fig. 5.7 shows that during the lateral loading (i) the sudden increase of normal displacements (ii) by 61 ±1 nm and 52 ± 1 nm is observed for the curves of type 1 and 2 respectively. There-fore, the failure observed in Fig. 5.6 occurs both in the direction of lateral and normal forces ap-plication. It should be noted that the previous sudden decrease of normal displacement by about 14 nm is detected for both types of curves. At the failure the bending of indenter shaft, which appears at the beginning of lateral force application as was mentioned above, decreases or disap-pears at all. The reason is that indenter moves together with sample material at the point of fail-ure event without overcoming friction force. As the result the decrease of normal displacement is observed.
At further lateral loading (iii) the normal displacement increases up to the maximum value due to indenter sliding. Further lateral unloading (iv) leads to the decreasing of normal displace-ment. However, after the removal of lateral force (v) the residual normal deformation is observed because of initial failure at lateral loading. It should be remarked that the value of residual de-formation for both types of curves is less than the sudden increase of normal displacement during the lateral loading. The residual normal deformation is 50 ± 1 nm for the curve of type 1 and 27
± 1 nm for the curve of type 2.
The failure can be detected by the observation of sudden change of lateral displacement in lateral force-displacement curve together with normal displacement in normal displacement-time curve. It was established that in the investigated example the critical lateral force for the failure is 14.7 ± 0.1 mN at the normal load of 400 mN.